### Jacopo Baima, Alessandro Erba*, Lorenzo Maschio, Claudio

### M. Zicovich-Wilson, Roberto Dovesi, and Bernard Kirtman

**Direct Piezoelectric Tensor of 3D Periodic**

**Systems through a Coupled Perturbed**

**Hartree–Fock**

**/Kohn–Sham Method**

DOI 10.1515/zpch-2015-0701

Received October 14, 2015; accepted November 9, 2015

**Abstract: A quasi-analytical theoretical method is devised, and implemented in**

the Crystal program, for calculation of the direct “proper” piezoelectric tensor of periodic systems including both the clamped-nuclei electronic and nuclear relaxation contributions. It is based on using the analytical Coupled-Perturbed-Hartree–Fock/Kohn–Sham (CPHF/KS) procedure to obtain dipole derivatives with respect to lattice deformations as well as internal coordinates. The sole nu-merical step required involves building the Hessian matrix through differentiation of analytical energy gradients. Two prototypical piezoelectric, non-ferroelectric, crystals, namelyZnOand𝛼-quartz, are used to demonstrate the accuracy and computational efficiency of our new scheme, which significantly improves upon the commonly used numerical Berry phase approach.

**Keywords: Piezoelectricity, Polarization in Solids, CPHF, CRYSTAL Program.**

||

**Dedicated to Professor Michael Springborg on the occasion of his 60**thbirthday

***Corresponding author: Alessandro Erba, Dipartimento di Chimica and Interdepartmental**

Centre NIS (Nanostructured Interfaces and Surfaces), Università di Torino, via Giuria 5, IT-10125 Torino, Italy, e-mail: [email protected]

**Jacopo Baima, Lorenzo Maschio: Dipartimento di Chimica and Interdepartmental Centre NIS**

(Nanostructured Interfaces and Surfaces), Università di Torino, via Giuria 5, IT-10125 Torino, Italy

**Claudio M. Zicovich-Wilson: Centro de Investigación en Ciencias, Universidad Autónoma del**

Estado de Morelos, Av. Universidad, 1001, Col. Chamilpa, 62209 Cuernavaca, Morelos, Mexico

**Roberto Dovesi: Dipartimento di Chimica and Interdepartmental Centre NIS (Nanostructured**

Interfaces and Surfaces), Università di Torino, via Giuria 5, IT-10125 Torino, Italy

**Bernard Kirtman: Department of Chemistry and Biochemistry, University of California, Santa**

**1 Introduction**

The phenomenon of piezoelectricity, i.e. the electric polarization (or dipole
mo-ment) that arises in certain solid materials as a response to an applied mechanical
force, has been known since the late 19th century [1]. However, it is only within
the past20 years, or so, that a thorough microscopic understanding of electric
polarization for periodic systems, which is our interest here, has been attained
and meaningful*ab initio calculations of piezoelectricity, as well as its converse*
(the mechanical strain induced by an applied field) [2–4], have become possible.
We now know that, although the electronic polarization may be regarded as a bulk
property, it is multivalued depending upon the surface charge [5,6]. In order to
ob-tain a unique value for the piezoelectricity (sometimes called the “proper”
piezo-electric response) one must evaluate/measure this property in terms of a voltage
rather than an electric field [5–8]. It is also now recognized that the nuclear
re-laxation contribution to piezoelectricity due to internal microscopic strain is
gen-erally comparable to, or even larger than, the purely electronic (clamped-nuclei)
term [9,10].

Given a satisfactory formalism for periodic systems (see Section2), the re-maining task is to develop an optimum computational algorithm with regard to accuracy and efficiency. On both grounds it is generally preferable to maximize the amount of analytical (versus numerical) differentiation occurring in the cal-culations. Recently, some of us have formulated, and implemented in the Crystal code [11], a fully analytical method for computing Born charges [12,13]. This pro-cedure is based on an analytical coupled perturbed Hartree–Fock/Kohn–Sham (CPHF/KS) treatment of the polarization along with analytical gradients of the field-dependent energy. As far as the clamped-nuclei contribution is concerned, the required polarization derivatives with respect to the external strain are evalu-ated through an extension of the CPHF/KS treatment utilized for the Born charges. In our evaluation of piezoelectric coefficients the so-called ionic contribution is, by far, the most costly part of the calculation due to the number of derivatives involved. What one requires are the clamped-nuclei (zero strain) derivatives of the polarization with respect to internal coordinates (i.e. the Born charges) and the derivatives of these internal coordinates with respect to the external strain vari-ables. The latter, in turn, are obtained through the Hessian matrix. In this paper the previous analytical calculation of Born charges is utilized in conjunction with a Hessian matrix that is obtained by numerical differentiation of analytical gra-dients with respect to atomic coordinates and lattice vector components [14–17]. Thus, our treatment of the ionic contribution is quasi-analytical. For a fully ana-lytical procedure the second derivatives should be obtained anaana-lytically as well.

Despite some techniques based on density-functional perturbation theory, proposed in the last two decades [18–20], the current most widely used approach to compute the piezoelectric response of crystals is the numerical Berry phase scheme [5,21,22]. The latter was first implemented in the Crystal code ten years ago [23,24] and has been fully automated in Crystal14 [25,26]. In these previ-ous implementations, the derivatives of the internal coordinates with respect to external strain variables, needed for the ionic contribution, were found by opti-mization of the internal structure at various strained geometries [25,27–32]. For good accuracy, such optimizations require very tight convergence, which implies relatively long computation times. The advantages of using numerical differenti-ation of analytical gradients instead are also documented in this paper.

The outline of our paper is as follows. Section2is devoted to our computa-tional strategy. The definition of the clamped-nuclei electronic and nuclear relax-ation contributions to the piezoelectric tensor is provided in Section2.1; the for-mulation of the analytical CPHF/KS scheme for calculation of both contributions to the “proper” piezoelectric tensor is developed in Section2.2; Voigt’s notation is introduced in Section2.3; and the main features of the standard Berry phase ap-proach are briefly recalled in Section2.4. Then the accuracy and computational efficiency of our method is documented in Section3, where it is also compared with the Berry phase approach, usingZnOand𝛼-quartz as test cases. Finally, our conclusions are presented in Section4.

**2 Computational strategy**

**2.1 Definition of the piezoelectric tensor**

The total “proper” direct piezoelectric response of a crystal can be represented by a third-rank tensor and is given by the sum of an electronic and a nuclear term,

**e = e**ele** _{+ e}**nuc

_{. The electronic term measures the variation of the current density}

**J**with strain when no nuclear relaxation is allowed (clamped-nuclei condition;

𝑢 = 0) [5]:
𝑒ele
𝑖𝑗𝑘 =
𝜕𝐽_{𝑖}
𝜕𝜖_{𝑗𝑘}_{}_{𝑢=0} = ∑𝛼
𝜕𝐽_{𝑖}
𝜕𝑎_{𝛼𝑗}𝑎𝛼𝑘
𝑢=0
. (1)

Here𝑖,𝑗,𝑘are Cartesian indices,**𝜖**is the symmetric second-rank pure strain tensor
and the𝑎_{𝛼𝑘}are Cartesian components of the three lattice vectors**a**_{𝛼},𝛼 = 1, 2, 3.
The second equality in Equation (1) arises from the expression for the effect of an

elastic deformation on the lattice parameters, i.e. [33]

𝑎

𝛼𝑗= ∑

𝑘

(𝛿_{𝑗𝑘}+ 𝜖_{𝑗𝑘})𝑎_{𝛼𝑘}, (2)

in which𝛿_{𝑗𝑘}is the Kronecker delta.

The nuclear relaxation contribution can be expressed as [9]:

𝑒nuc
𝑖𝑗𝑘 = _{𝑉}1 ∑
𝑠 𝑍
∗
𝑖𝑠
d𝑢_{𝑠}
d𝜖_{𝑗𝑘}, (3)

where**𝑉 = a**_{1}**⋅(a**_{2}**×a**_{3}) is the cell volume, the𝑢_{𝑠}are3𝑁 −3fractional coordinates
(𝑁being the number of atoms per cell) obtained from the3𝑁atomic fractional
co-ordinates by orthogonalization to the three translations along ̂𝑥, ̂𝑦and ̂𝑧, and**Z**∗
is the Born atomic charge tensor defined in terms of the resulting set of fractional
atomic coordinates:

𝑍∗

𝑖𝑠= 𝜕

2_{𝐸}𝑇𝑂𝑇

𝜕E_{𝑖}𝜕𝑢_{𝑠}. (4)

In the latter relationE_{𝑖}is a Cartesian component of the applied electric field and

𝐸𝑇𝑂𝑇_{the total energy of the system (to be given an explicit expression below).}

**2.2 The coupled-perturbed approach**

**2.2.1 Electronic Term**

The electronic contribution to the “proper” piezoelectric tensor defined in
Equa-tion (1) can be expressed in terms of the total polarization**P**as [5]:

𝑒ele
𝑖𝑗𝑘= _{𝜕𝜖}𝜕𝐽𝑖
𝑗𝑘
𝑢=0
= 𝜕𝑃𝑖
𝜕𝜖𝑗𝑘
𝑢=0
+ 𝑃𝑖𝛿𝑗𝑘− 𝑃𝑘𝛿𝑖𝑗, (5)

where the first term on the right-hand-side can be understood as the electronic contribution to the “improper” piezoelectric tensor. By expressing the polariza-tion in terms of total energy derivatives, and by exploiting the second equality in Equation (1), one gets:

𝜕𝐽𝑖
𝜕𝜖𝑗𝑘
𝑢=0
= 1
𝑉∑𝛼 𝑎𝛼𝑘
𝜕2_{𝐸}𝑇𝑂𝑇
𝜕E𝑖𝜕𝑎𝛼𝑗
𝑢=0
− 𝑃_{𝑘}𝛿_{𝑖𝑗}. (6)

The second derivatives in the term on the rhs of Equation (6) are the same as the components of the Born charge tensor in (4) except that differentiation with spect to internal atomic positions has been replaced by differentiation with re-spect to the lattice parameters. Here we develop an expression for the latter by

extending the analytical CPHF/KS approach recently presented for calculation of the Born tensor by Maschio, Kirtman, Orlando and Rérat (MKOR) [12]. Extensive reference will also be made to the work by Doll, Dovesi and Orlando (DDO) on the development, and implementation in the Crystal program, of analytical energy gradients with respect to lattice distortions [16].

We start with the Hartree–Fock expression (the extension to Kohn–Sham DFT
can be found in MKOR) for the total energy of a periodic system in the presence of
an electric field:
𝐸𝑇𝑂𝑇 _{=}_{Tr}_{([𝐻 +} 1
2(𝐵 + 𝑇 + 𝑆𝑞) + ∑_{𝑙} E𝑙𝛺𝑙] 𝐷)
+ 𝐸nuc_{+ ∑}
𝑙,𝑚,𝐴
E_{𝑙}𝜁_{𝐴}R𝐴_{𝑚}𝛿_{𝑙𝑚}. (7)

In this expression Tr signifies the trace and𝐻, 𝐵, 𝑇, 𝑆, 𝛺_{𝑙} and𝐷 are direct
space matrices in an atomic orbital (AO) representation. Specifically,𝐻is the core
Hamiltonian,𝑆the overlap,𝐵the electron–electron interaction term (which
in-volves evaluation of two-electron integrals), and𝑇the Ewald infinite summation
contribution to the electron–electron interaction (which depends upon the
den-sity matrix𝐷). Furthermore,R𝐴_{𝑚}= ∑_{𝛽}𝑓_{𝐴,𝛽}𝑎_{𝛽𝑚}is the position of atom𝐴along the
Cartesian direction𝑚with fractional coordinate𝑓_{𝐴,𝛽},𝜁_{𝐴}is the nuclear charge of
atom𝐴and𝐸nucthe nuclear-nuclear interaction energy.

Two quantities,𝛺_{𝑙}and𝑞, in Equation (7) require a more detailed explanation.

𝛺_{𝑙}is the AO matrix representation, in direct space, for the𝑙Cartesian component
of an operator,**𝛺(k)**̂ , which determines the interaction of the electrons with the
external electric field. For an infinite periodic system it is defined as [34–38]:

̂

**𝛺(k) = 𝚤𝑒𝚤k⋅r**∇** _{k}**𝑒

**−𝚤k⋅r**. (8) The properties of this matrix, which is central to our approach, have been exten-sively discussed in previous papers by some of us [12,39,40]. If the matrix of crystalline orbital eigenvectors

**𝐶(k)**is expanded as a Taylor series in the field components:

**𝐶(k) = 𝐶**(0)

**(k) + ∑**𝑙 E𝑙𝐶(E𝑙)

**(k)**+ ∑ 𝑙,𝑚 E𝑙E𝑚𝐶(E𝑙,E𝑚)

**(k) + . . .**(9)

then, the zeroth-order matrix representation of the operator (8) may be written as [12]:

𝛺(0)_{𝑙} **(k) = 𝑀**_{𝑙}**(k)**

**+ 𝚤𝑆(k)𝐶**(0)_{(k)𝑄}

where𝑀_{𝑙}**(k) = 𝛯**_{𝑙}**(k) + 𝚤𝑆**(𝑘𝑙)**(k)**_{. Here}𝛯

𝑙**(k)**is the matrix representing the

com-ponent of the electron position coordinate along𝑙and𝑆(𝑘𝑙)**(k)**_{is the derivative of}

the AO overlap matrix**𝑆(k)**with respect to the wave vector component𝑘_{𝑙}[41]. The
crystal orbital (CO) matrix𝑄_{𝑙}**(k)**is defined by:

𝜕

𝜕𝑘_{𝑙}𝐶(0)**(k) = 𝐶**(0)**(k)𝑄**𝑙**(k).** (11)

Note that this CO matrix contains both real and imaginary parts. It has been shown previously that the imaginary diagonal components, which contribute to the dipole moment, are only determined up to an integer multiple of the unit cell length along each of the crystal axes [38,42,43].

In Equation (7),𝑞is the (scalar) value of the spheropole. The spheropole term arises only in 3D periodic systems. It occurs because the charge distribution is ap-proximated by a model in the long range and it is needed in order to guarantee that the average of the electrostatic potential vanishes [44]. We note that𝑞 de-pends upon the density matrix,𝑞 =Tr(𝐷Q), whereQis the matrix of spheropolar integrals whose explicit form can be found elsewhere [16,44].

Following the scheme of the MKOR treatment, it is convenient to begin with the expression for the analytical gradient of𝐸𝑇𝑂𝑇with respect to cell parameters (see Equation (6) in DDO) and, then, differentiate this expression with respect to the electric field:

𝜕𝐸𝑇𝑂𝑇
𝜕𝑎_{𝛼𝑗} _{}_{𝑎}0
= 𝜕𝐸nuc
𝜕𝑎_{𝛼𝑗} _{}_{𝑎}0
+Tr([1
2(B(𝑎𝛼𝑗)+ T(𝑎𝛼𝑗)+ q(𝑎𝛼𝑗)𝑆 + 𝑞𝑆(𝑎𝛼𝑗))
+∑
𝑙
E𝑙𝛺(𝑎𝑙 𝛼𝑗)+ 𝐻(𝑎𝛼𝑗)] 𝐷 − 𝑆(𝑎𝛼𝑗)𝐷𝑊)
𝑎0
+ ∑
𝐴,𝑙
E_{𝑙}𝛿_{𝑙𝑗}𝜁_{𝐴}𝑓_{𝐴,𝛼}, (12)

The subscript𝑎0here indicates that the quantity in question is evaluated for
equi-librium cell parameters. As customary in the evaluation of energy gradients [45],
the eigenvalue-weighted density matrix𝐷_{𝑊}has been introduced in order to avoid
calculating derivatives of the CO coefficients.

In Equation (12) the first term on the rhs is not trivial to evaluate. However, it
does not depend on the electric field and is, therefore, not relevant for the present
discussion. The derivatives that appear in the second term can be treated, for the
most part, in almost exactly the same way as those that occur for the Born
ten-sor in MKOR except that now the lattice parameters are varied with the internal
vibrational displacements held fixed rather than the other way around. In
partic-ular,B(𝑎𝛼𝑗)_{,}T(𝑎𝛼𝑗)_{and}q(𝑎𝛼𝑗)_{are derivatives of the electron-electron interaction and}

spheropole terms𝐵,𝑇and𝑞, taken by keeping the density matrix constant; they
correspond to Equations (30)–(32) in MKOR. That leaves𝐻(𝑎𝛼𝑗)_{, the derivative of}

the kinetic energy and electron-nuclear interaction contributions, as well as𝑆(𝑎𝛼𝑗)_{,}

neither of which contain the density matrix.

There are three terms that require further elaboration. One of them is the
spheropole derivativeq(𝑎𝛼𝑗)_{, which contains an additional term with respect to the}

Born tensor case (see Equation (48) of DDO):

q(𝑎𝛼𝑗)=_{Tr}(𝐷Q(𝑎𝛼𝑗)) + 𝑞
𝑉

𝜕𝑉

𝜕𝑎_{𝛼𝑗}. (13)

The others are the two terms in Equation (12) that depend explicitly on the field.
At variance with the Born tensor, when the lattice parameters are varied these
two terms do not yield a unique value for the derivative. The last term in
Equa-tion (12) describes the interaction between the external field and the nuclear
charges, whereas the interaction of the electrons with the external field is given
by∑_{𝑙}E_{𝑙}𝛺_{𝑙}(𝑎𝛼𝑗). Each of these terms, individually, depends upon the choice of the
origin and the unit cell, which leads to different possible values depending upon
the surface termination of the lattice of point charges [5]. However, this
depen-dence cancels except for a contribution that arises from the diagonal imaginary
elements of𝑄_{𝑙}[7,38]:

1
2𝑛𝑘 ∑**k**

Tr(𝚤 (𝑄(𝑎_{𝑙}𝛼𝑗)**(k) − 𝑄**(𝑎_{𝑙} 𝛼𝑗)†**(k)) 𝑛)**

𝑎= 𝑒𝛿0 𝑙𝑗𝑁𝛼, (14)

where𝑛is the diagonal occupation number matrix with eigenvalues equal to0
for virtual orbitals and1(or2in closed shell systems) for occupied orbitals,𝑛_{𝑘}
is the number of**k**-points included in the summation,𝑒is the magnitude of the
electron charge and𝑁_{𝛼}is an arbitrary integer (or even integer for closed-shell
systems). Apart from normalization, the term on the lhs here is the same as in
Equation (39) of MKOR except, again, that the derivatives are with respect to
ex-ternal strain rather than inex-ternal atomic displacements. An alternative derivation
is given in Reference [13]. Physically, this term accounts for the dipole moment
generated by transfer of a quantized number of charges,𝑁_{𝛼}, per unit cell between
opposite surfaces [5,6]. However, we note that the polarization𝑃_{𝑙}also contains
a contribution∑_{𝛽}𝑒𝑁_{𝛽}𝑎_{𝛽𝑙}due to the charge transfer. Indeed, when the “proper”
piezoelectric tensor, the subject of this paper, is determined by subtracting out

𝑃𝑘𝛿𝑖𝑗(see Equation6) the charge transfer terms cancel out. On the contrary, such

cancellation does not occur for the “improper” piezoelectric tensor, which is given by the first term on the rhs of Equation (5) and is also physically observable, as discussed elsewhere for one-dimensional periodic systems [6].

By differentiating Equation (12) with respect to the electric field we obtain the analogue of Equation (48) in MKOR:

𝜕
𝜕E𝑖
𝜕𝐸𝑇𝑂𝑇
𝜕𝑎𝛼𝑗
E=0,𝑎0
=Tr([𝐻(𝑎𝛼𝑗)+ B(𝑎𝛼𝑗)+ 1
2T(𝑎𝛼𝑗)] 𝐷(E𝑖)
+ [1
2(q(𝑎𝛼𝑗)𝑆+ T(𝑎𝛼𝑗))
(E𝑖_{+ 𝑀}) (𝑎𝛼𝑗)
𝑖 ] 𝐷(0)− 𝑆(𝑎𝛼𝑖)𝐷(E𝑖
)
𝑊 )
𝑎0
+ ∑
𝐴
𝜁_{𝐴}𝑓_{𝐴,𝛼}𝛿_{𝑖𝑗}+ 𝑒𝛿_{𝑖𝑗}𝑁_{𝛼}, (15)
where𝐷(E_{𝑊}𝑖)is a modified form of the electric field derivative of the
eigenvalue-weighted density matrix (see Equation 45 of MKOR). The modification, indicated
by thesuperscript, entails subtracting out the terms containing𝑄from the
La-grange multiplier matrix that appears in𝐷. Following through on the terms
sin-gled out in connection with Equation (12), we note that the spheropole term
be-comes (see Equation13):

(q(𝑎𝛼𝑗))(E𝑖)=_{Tr}(𝐷Q(𝑎𝛼𝑗))(E𝑖)+ 𝑞

(E𝑖) 𝑉

𝜕𝑉

𝜕𝑎_{𝛼𝑗}. (16)

In addition, the two terms on the rhs that arise from𝛺_{𝑖}in Equation (12), namely

𝑀(𝑎𝛼𝑗)

𝑖 𝐷(0)(𝑀𝑖is the hermitized version of𝑀𝑖) and𝛿𝑖𝑗𝑁𝛼, as well as the nuclear

contribution to the dipole moment (next to last term on rhs of Equation15) all
depend upon the origin and shape of the lattice cell. However, this dependence
does not occur in the “proper” piezoelectric effect since, after the sum is taken,
what remains is canceled by the−𝑃_{𝑘}𝛿_{𝑖𝑗}term in Equation (6).

**2.2.2 Nuclear relaxation term**

The nuclear relaxation contribution to the “proper” piezoelectricity is given by
Equation (3). In fact, there is no distinction between “proper” and “improper”
for this term because the atomic Born charge tensor**Z**∗is independent of surface
charges as noted in MKOR. In the present approach**Z**∗is computed analytically
through a CPHF/KS strategy [12,13], and is obtained in conjunction with the
deter-mination of the clamped-nuclei electronic term. That leaves the d𝑢_{𝑠}/d𝜖_{𝑗𝑘}
deriva-tives in Equation (3). They can be obtained in either of two ways: i) optimization of
the internal geometry at strained configurations or ii) from the full Hessian matrix

**H**of energy second derivatives with respect to both fractional atomic
displace-ments and lattice deformations (with a truncation to quadratic terms in the
Tay-lor’s expansion of the energy) [20]. We have found that ii) is preferable, as will be

documented in Section3.2. In that procedure the following relation is utilized:
d𝑢_{𝑠}
d𝜖_{𝑗𝑘} = −
3𝑁−3
∑
𝑠_{=1}
𝐻_{𝑗𝑘,𝑠}× (𝐻−1)_{𝑠}_{𝑠}, (17)
in which
𝐻_{𝑗𝑘,𝑠} = ( 𝜕
2_{𝐸}
𝜕𝜖_{𝑗𝑘}𝜕𝑢_{𝑠}) ,
(18)
and(𝐻−1)_{𝑠}_{𝑠}is an element of the inverse of the atomic Hessian:

𝐻𝑠_{𝑠}= ( 𝜕

2_{𝐸}

𝜕𝑢_{𝑠}𝜕𝑢_{𝑠}) .

(19) In the present implementation, the elements of the Hessian matrix are com-puted as numerical derivatives of analytical energy gradients. Either a two-point or three-point formula is employed in obtaining the numerical derivatives with the analytical gradients computed at the equilibrium configuration and at one or two non-equilibrium, i.e. displaced or strained, configurations for Equations (19) and (18), respectively. As both the3𝑁 − 3fractional atomic coordinates𝑠and the

6symmetry-independent lattice deformations𝜖_{𝑗𝑘}(the pure strain tensor𝜖being
symmetric) imply global atomic displacements, non-equilibrium configurations
are defined in terms of the largest induced Cartesian atomic displacement𝛿(by
default𝛿 = 0.004 bohr). If mass-weighted coordinates are used instead of𝑢_{𝑠}, then
by diagonalizing the atomic Hessian matrix (Equation (19)), the total nuclear
re-sponse𝑒nuccan be expressed as a sum of normal mode-specific contributions:

𝑒nuc
𝑖𝑗𝑘 = −_{𝑉}1 ∑
𝑝 𝑍
∗
𝑖𝑝
𝐻_{𝑗𝑘,𝑝}
𝜔2
𝑝
, (20)

where𝑝 = 1, . . ., 3𝑁 − 3labels each vibration normal mode and𝜈_{𝑝}is the
corre-sponding vibration frequency.

**2.3 Voigt’s notation**

As the pure strain𝜖is a symmetric second-rank tensor, there are six independent
components𝜖_{𝑗𝑘}. It is convenient to adopt Voigt’s notation, which maps the two
Cartesian index notation(𝑗𝑘)into a one index notation(𝑣), where𝑣 = 1 ≡ 𝑥𝑥,

𝑣 = 2 ≡ 𝑦𝑦,𝑣 = 3 ≡ 𝑧𝑧,𝑣 = 4 ≡ 𝑦𝑧,𝑣 = 5 ≡ 𝑥𝑧, and𝑣 = 6 ≡ 𝑥𝑦[46]. Accordingly, the third-rank direct piezoelectric tensor can be represented as a two-index quantity:

𝑒_{𝑖𝑗𝑘}→ 𝑒_{𝑖𝑣}. (21)

**2.4 The Berry phase approach**

Within the modern theory of polarization [5,21,22], the direct “proper” piezoelec-tric constants of 3D crystals can be obtained from derivatives of the numerical Berry phase𝜑with respect to the strain as:

𝑒𝑖𝑣= _{2𝜋𝑉}𝑒 ∑
𝛼 𝑎𝛼𝑖

d𝜑_{𝛼}

d𝜖_{𝑣}, (22)

where 𝜑_{𝛼} represents the Berry phase along the **a**_{𝛼} lattice vector. In the
fully-automated implementation available in the Crystal14 version of the program,
the derivatives in Equation (22) were obtained numerically by finite differences
over Berry phases computed at𝑁_{𝑝} strained configurations, which span a strain
amplitudeΔ(by default,𝑁_{𝑝}= 3andΔ = ±1.5%of the unstrained lattice
parame-ters) [25,26]. The effect of nuclear relaxation is evaluated numerically by allowing
internal coordinates𝑢_{𝑠}to relax at strained configurations, which corresponds to
procedure i) in Section2.2.2. If geometry optimizations at strained configurations
are avoided, the purely electronic contribution is computed, which would
corre-spond to evaluating partial instead of total derivatives in Equation (22).

**3 Results and discussion**

In this section, we document and discuss the accuracy and efficiency of the
ana-lytical scheme (based on the CPHF/KS method) for the quantum-mechanical
eval-uation of the “proper” direct piezoelectric tensor of crystals. A comparison with
the commonly used numerical approach (based on the Berry phase method), as
in Crystal14, is also presented in order to demonstrate the computational
advan-tages of the present formulation/implementation. Since the electronic and
nu-clear relaxation contributions to the total piezoelectric response are computed
following distinct computational strategies we shall discuss these terms
sepa-rately. For this analysis, two prototypical non-ferroelectric piezoelectric materials
are considered: hexagonal zinc oxide,ZnO, and trigonal𝛼-quartz,𝛼-SiO_{2}. The
former has three symmetry-independent piezoelectric constants:𝑒_{15},𝑒_{31}and𝑒_{33},
whereas the latter has two:𝑒_{11}and𝑒_{14}.

For our purposes here it is convenient to use the CPKS treatment with
the generalized gradient PBE [47] functional. We have chosen a local basis
set of atom-centered Gaussian-type functions with the following contractions:
(8𝑠)(64111𝑠𝑝)(41𝑑) for Zn, (8𝑠)(411𝑠𝑝)(1𝑑) forO, and (8𝑠)(841𝑠𝑝)(1𝑑) for Si.
A tight threshold of10−10hartreeis set for the energy convergence of the field-free
self-consistent-field (SCF) procedure. The convergence threshold𝑇_{𝛼}for the SCF

procedure within the CPKS method will be explicitly discussed in the next sub-sections. In evaluating the long-range electron-electron Coulomb interactions the maximum order of shell multipoles is set to6(seePOLEORDR keyword in the Crys-tal14 manual [48]). The exchange-correlation contribution to the Fock matrix is evaluated by numerical integration over the unit cell volume. Radial and angular points of the integration grid were generated by Gauss-Legendre radial quadra-ture and a Lebedev two-dimensional angular distribution. In the present work, a pruned grid with99radial points and a maximum of1454angular points is used, which corresponds to the densest grid (seeXXLGRID keyword in the Crys-tal14 manual) [48] among the pre-defined ones. Other computational parameters will be discussed in the following sub-sections.

**3.1 Computational parameters for electronic term**

We consider, first, the electronic “clamped-nuclei” piezoelectric constants. They
are reported in Table1as a function of two computational parameters: the
shrink-ing factor𝑆, which determines the number of**k**-points sampled in reciprocal
space, and the tolerances𝑇_{𝑖}(i.e.10−𝑇𝑖_{), which govern the truncation of the }

in-finite Coulomb and exchange series. In the Crystal program there are five such
thresholds that are set here to𝑇_{1}= 𝑇_{2}= 𝑇_{3}= 𝑇_{4}= 1

2𝑇5= 𝑇[48].

It is seen in the table that the calculated piezoelectric coefficients of the two crystals are quite insensitive to the values of both computational parameters ex-cept for small values of𝑆. In that case, the CP approach is more sensitive than the BP approach forZnO, whereas the situation is reversed for𝛼-quartz, although the effect is much smaller. Both approaches converge nicely to the same limiting values. ForZnOthe analytical CP coefficients are converged to three significant figures at𝑆 = 9,𝑇 = 9while the numerical BP coefficients are fully converged at

𝑆 = 12,𝑇 = 8. The corresponding parameters for𝛼-quartz are𝑆 = 3,𝑇 = 5for the CP method and𝑆 = 6,𝑇 = 5for the BP method.

We turn now to the algorithm-specific computational parameters. The main computational parameter to explore for the CP analytical strategy is the threshold

𝑇𝛼(i.e.10−𝑇𝛼), which controls the convergence of the self-consistent CPKS

equa-tions in terms of components of the polarizability tensor**𝛼**. In the upper part of
Ta-ble2, this parameter is considered in the range100–10−4. For both systems,𝑇_{𝛼}= 2
provides converged coefficients to three significant figures. In the BP approach, as
recalled in Section2.4, the piezoelectric constants are determined via numerical
derivatives of the Berry phase with respect to the strain. The derivatives are
calcu-lated by finite differences with the Berry phases evaluated at𝑁_{𝑝}equally spaced
points with a maximum strain amplitudeΔ(the latter is expressed as a percent of

**Table 1: The clamped-nuclei electronic contribution to the symmetry-independent piezoelectric**

constants ofZnO and 𝛼-quartz for the Berry phase (BP) and CPKS (CP) approaches as a function
of the shrinking factor𝑆 and truncation tolerance 𝑇 of the infinite Coulomb series. All values in
units of_{C/m}2.
ZnO S_{= 3} S_{= 6} S_{= 9} S_{= 12}
BP CP BP CP BP CP BP CP
𝑒ele
15 0.315 0.391 0.316 0.323 0.318 0.319 0.319 0.319
𝑒ele
31 0.309 0.356 0.306 0.309 0.306 0.307 0.307 0.307
𝑒ele
33 −0.635 −0.647 −0.619 −0.617 −0.616 −0.615 −0.615 −0.615
T= 6 T= 7 T= 8 T= 9
BP CP BP CP BP CP BP CP
𝑒ele
15 0.319 0.320 0.319 0.320 0.319 0.320 0.319 0.319
𝑒ele
31 0.306 0.308 0.307 0.307 0.307 0.307 0.307 0.307
𝑒ele
33 −0.614 −0.612 −0.614 −0.613 −0.615 −0.614 −0.615 −0.615
𝛼-SiO2 S_{= 2} S_{= 3} S_{= 6} S_{= 9}
BP CP BP CP BP CP BP CP
𝑒ele
11 −0.142 −0.147 −0.144 −0.145 −0.145 −0.145 −0.145 −0.145
𝑒ele
14 0.068 0.074 0.071 0.073 0.073 0.073 0.073 0.073
T= 5 T= 6 T= 7 T= 8
BP CP BP CP BP CP BP CP
𝑒ele
11 −0.145 −0.145 −0.145 −0.145 −0.145 −0.145 −0.145 −0.145
𝑒ele
14 0.073 0.073 0.073 0.073 0.073 0.073 0.073 0.073

the equilibrium lattice parameter). The lower part of Table2documents the
com-bined effect of𝑁_{𝑝}andΔ. Overall, a very satisfactory numerical stability of the
computed numerical derivatives is found.

**3.2 Computational parameters for nuclear relaxation term**

We now proceed to examine the effect of the (algorithm-specific) computational
parameters on the nuclear relaxation contribution to the piezoelectric coefficients
of ZnOand𝛼-quartz. The computational parameters discussed in Section 3.1
(namely𝑆,𝑇,𝑇_{𝛼},𝑁_{𝑝}andΔ) are kept fixed at values that guarantee full
conver-gence of the clamped-nuclei electronic term in both strategies.

The nuclear relaxation factor d𝑢_{𝑠}/d𝜖_{𝑣}in Equation (3) is accounted for
differ-ently in the two approaches. Within the BP approach, geometry optimizations are
performed at strained lattice configurations through a quasi-Newton scheme [27].

**Table 2: Effect of algorithm-specific computational parameters on the clamped-nuclei electronic**

piezoelectric constants ofZnO and 𝛼-quartz. For the CP approach, 𝑇_{𝛼}is the threshold for
convergence of the CPKS equations; for the BP approach,Δ is the strain amplitude and 𝑁𝑝is the
number of points used to numerically evaluate the Berry phase derivative with respect to strain.

CP 𝑇𝛼 0 1 2 3 4 ZnO 𝑒ele 15 0.320 0.319 0.319 0.319 0.319 𝑒ele 31 0.347 0.322 0.307 0.307 0.307 𝑒ele 33 −0.578 −0.601 −0.615 −0.615 −0.615 𝛼-SiO2 𝑒ele11 −0.153 −0.145 −0.145 −0.145 −0.145 𝑒ele 14 0.062 0.074 0.073 0.073 0.073 BP 𝑁𝑝 3 3 5 5 5 Δ ±1% ±1.5% ±1% ±1.5% ±2% ZnO 𝑒ele 15 0.319 0.319 0.319 0.319 0.319 𝑒ele 31 0.307 0.307 0.307 0.307 0.307 𝑒ele 33 −0.616 −0.615 −0.614 −0.615 −0.616 𝛼-SiO2 𝑒ele 11 −0.145 −0.145 −0.145 −0.145 −0.145 𝑒ele 14 0.073 0.073 0.073 0.073 0.073

A threshold parameter𝑇_{𝐺}(i.e.10−𝑇𝐺_{) is used to determine the convergence of the}

geometry optimization process based on the root mean square value of the
gra-dients. In the CP approach, the same factor is evaluated though Equation (17) by
constructing the Hessian matrix**H**from finite differences of analytical gradients
evaluated at𝑛_{𝑝}displaced/distorted configurations with a displacement step𝛿.

Table3 documents the effect of the above parameters on computed total (clamped-nuclei electronic plus nuclear relaxation) piezoelectric coefficients of

ZnOand𝛼-quartz. At the outset we stress the fact that the nuclear relaxation
contribution is dominant in every case so that total values of all piezoelectric
co-efficients𝑒_{𝑖𝑣}are of opposite sign to the corresponding clamped-nuclei electronic
contribution𝑒ele_{𝑖𝑣} reported in previous tables. The𝑇_{𝐺}threshold used for the BP
method is explored in the range3 ⋅ 10−4–1 ⋅ 10−5. Although the computed
coeffi-cients are not dramatically affected by the threshold value, the convergence is very
slow. This observation is based on the fact that the third significant figure varies
between𝑇_{𝐺} = 0.3and0.1. For𝛼-quartz, in particular, the coefficient values are
probably not fully converged. In general, then, tighter values than1 ⋅ 10−5might
need to be used for𝑇_{𝐺}, which would require a tightening of many other

**computa-Table 3: Effect on the total piezoelectric constants of**ZnO and 𝛼-quartz of the algorithm-specific

computational parameters related to the nuclear relaxation term. For the CP strategy, the number𝑛𝑝of displaced/deformed configurations and the step 𝛿 (in bohr) used in the

construction of the Hessian matrix from finite differences of analytical gradients are considered. For the BP strategy, the threshold𝑇𝐺(in units of10−4a.u.) controlling the convergence of the geometry optimizations in terms of the root mean square of the gradients is explored.

CP 𝑛𝑝 2 2 3 3 3 𝛿 0.004 0.008 0.004 0.006 0.008 ZnO 𝑒15 −0.497 −0.497 −0.497 −0.497 −0.496 𝑒31 −0.593 −0.598 −0.590 −0.589 −0.589 𝑒33 1.148 1.147 1.148 1.148 1.148 𝛼-SiO2 𝑒11 0.188 0.188 0.190 0.190 0.190 𝑒14 −0.068 −0.070 −0.067 −0.067 −0.067 BP 𝑇𝐺 3 1 0.6 0.3 0.1 ZnO 𝑒15 −0.490 −0.497 −0.497 −0.498 −0.498 𝑒31 −0.584 −0.589 −0.589 −0.590 −0.589 𝑒33 1.146 1.146 1.146 1.149 1.149 𝛼-SiO2 𝑒11 0.196 0.195 0.194 0.194 0.193 𝑒14 −0.062 −0.063 −0.064 −0.064 −0.065

tional parameters (such as the DFT numerical integration grid, the tolerances𝑇_{𝑖},
etc.) to ensure the necessary numerical accuracy.

With regard to the CP approach, Table3shows that the amplitude of the step𝛿
has a very small effect on most piezoelectric coefficients. On the contrary, passing
from a two-point formula𝑛_{𝑝}= 2to a three-point formula𝑛_{𝑝} = 3in constructing
the Hessian leads to a noticeable improvement of the nuclear relaxation term (in
particular, for the𝑒_{31} coefficient ofZnOand for both coefficients of𝛼-quartz).
When the two overall strategies are compared with each other, small differences in
the calculated coefficients are observed. These differences lie within the expected
range of round-off error due to the numerical differentiations involved in both the
CP and BP procedures.

**Table 4: Wall-clock time (in minutes) of the calculation, running in parallel mode on**24

processors, of the electronic clamped-nuclei term of the full piezoelectric tensor ofZnO and 𝛼-quartz, as a function of the algorithm-specific computational parameters 𝑇𝛼and𝑁𝑝for the CP and BP approaches, respectively.

CP 𝑇𝛼 0 1 2 3 ZnO 7.1 7.8 8.7 9.3 𝛼-SiO2 7.9 9.8 11.0 12.6 BP 𝑁𝑝 3 5 7 9 ZnO 47 67 88 108 𝛼-SiO2 55 83 111 139

**3.3 Computational performance**

In this section we compare the computational performance (in terms of required wall-clock time) of the two approaches for determining the total direct third-rank piezoelectric tensor ofZnOand𝛼-quartz. Although symmetry can be utilized in both schemes, it has not yet been implemented for the CP procedure. Thus, to enable a fair comparison here, symmetry was not exploited in either case.

Table4reports the wall-clock time required to run calculations (in parallel
over24processors) of the clamped-nuclei electronic term including, as well, the
Born charges needed for the nuclear relaxation term. For the clamped-nuclei
elec-tronic term there are just two algorithm-specific computational parameters that
need to be considered, namely𝑇_{𝛼}for CP and𝑁_{𝑝}for BP (the step sizeΔdoes not
affect timings). From inspection of the table, a couple of inferences can be made:
i) the CP analytical scheme is less costly than the numerical BP one (roughly by
a factor of5for both crystals if optimal parameters are considered, i.e.𝑇_{𝛼}= 2and

𝑁𝑝 = 3); ii) the computational cost only slightly increases for the CP scheme as

a function of𝑇_{𝛼}(increasing by about31%passing from𝑇_{𝛼}= 0to𝑇_{𝛼}= 3).
The relative performance of the two schemes for the nuclear relaxation term
may be discerned from Table5, which reports the wall-clock time of the total
cal-culation as well as the difference (in parentheses) between the total time and that
required for computation of the clamped-nuclei electronic term. The latter is taken
as the time for computation of the nuclear relaxation contribution. Given that
within the CP scheme Born charges are computed along with the electronic
con-tribution, the numbers in parentheses for both schemes essentially correspond
to the times required to compute d𝑢_{𝑠}/d𝜖_{𝑗𝑘}. From the table we see that: i)

**Compu-Table 5: Wall-clock time (minutes), when running in parallel mode on**24 processors, for

calculation of the total (clamped-nuclei electronic plus nuclear relaxation) piezoelectric tensor
ofZnO and 𝛼-quartz. Values are reported as a function of the algorithm-specific computational
parameters_{𝑛𝑝}and_{𝑇}_{𝐺}for the CP and BP approaches, respectively. In parentheses, the
difference between the wall-clock time of a total calculation and a clamped-nuclei electronic
calculation is reported.
CP
𝑛𝑝 2 3
ZnO 34 57
(_{25)} (_{48)}
𝛼-SiO2 67 125
(56) (114)
BP
𝑇𝐺 3 1 0.6 0.3
ZnO 114 142 152 183
(_{67)} (_{95)} (_{105)} (_{136)}
𝛼-SiO2 165 176 182 196
(110) (121) (127) (141)

tation of the nuclear relaxation term takes much longer than the clamped-nuclei
electronic term (a greater fraction of the total for CP than for BP); ii) For the CP
strategy, passing from𝑛_{𝑝} = 2to𝑛_{𝑝} = 3in the construction of the Hessian matrix
implies an increase of the computation time by roughly a factor of 2, as expected;
for the BP strategy tightening𝑇_{𝐺}gradually increases the wall-clock time, up to
a factor of2.4(ZnO) for the range of𝑇_{𝐺}considered; iii) Evaluation of the nuclear
relaxation term is faster with the CP approach. Based on the least expensive
com-putational settings in both cases, for example, we see that25 minis required for
the CP scheme versus67for the BP method in the case ofZnO; the
correspond-ing times for𝛼-quartz are67and165 min, respectively; iv) the CP quasi-analytical
strategy always takes considerably less time to compute the total tensor than the
BP one (more so forZnOthan𝛼-quartz).

**4 Conclusions**

We have developed a new quasi-analytical method for computation of the “proper” piezoelectric tensor of crystals including both clamped-nuclei electronic

TSaPlease add place of publication.

Editor’s or typesetter’s annotations (will be removed before the final TEX run) and nuclear relaxation contributions. This method, which has been implemented in the Crystal code, is based on extending a recently presented CPHF/KS proce-dure for obtaining dipole derivatives and also on numerical differentiation of an-alytical gradients to obtain the Hessian matrix. Our strategy is compared with the commonly used Berry phase approach in terms of accuracy, numerical stability and computational performance. Using PBE calculations onZnOand𝛼-quartz, the present quasi-analytical strategy is documented to be an optimal alternative to the numerical Berry phase approach. Moreover, a fully analytical procedure can be envisioned – it would require analytical determination of the Hessian.

Our present implementation does not take full advantage of symmetry as yet. However, work is currently in progress to overcome this limitation, which exploits features already present in the Crystal code. The overall treatment presented here can be extended to other properties requiring higher-order derivatives with respect to electric fields, such as photo-elasticity and piezo-optics. We intend to carry out these further developments in the near future.

**Acknowledgement: CMZW thanks the Mexican Conacyt for financial support**

through project CB-178853.

**References**

1. J. Curie and P. Curie, Comptes Rendus**91 (1880) 383.**

*2. M. Springborg, B. Kirtman, and J. Vargas, in: Advances in Quantum Methods and *

*Applica-tions in Chemistry, Physics, and Biology, vol. 27 of Progress in Theoretical Chemistry and*
*Physics, M. Hotokka, E. J. Brandas, J. Maruani, G. Delgado-Barrio (Eds.), Springer *

Interna-tional Publishing,TSa_{(2013), pp. 331–348.}

3. A. Sayede, E. Bruyer, and M. Springborg, Phys. Rev. B**86 (2012) 125136.**

4. M. Springborg, B. Kirtman, Y. Dong, and V. Tevekeliyska, AIP Conf. Proc.**1461 (2012) 116.**

5. D. Vanderbilt, J. Phys. Chem. Solids**61 (2000) 147.**

6. M. Springborg, V. Tevekeliyska, and B. Kirtman, Phys. Rev. B**82 (2010) 165442.**

7. M. Springborg and B. Kirtman, Theor. Chem. Acc.**130 (2011) 687.**

8. I. Souza, J. Íñiguez, and D. Vanderbilt, Phys. Rev. Lett.**89 (2002) 117602.**

9. G. Saghi-Szabo, R. E. Cohen, and H. Krakauer, Phys. Rev. Lett.**80 (1998) 4321.**

10. A. Dal Corso, M. Posternak, R. Resta, and A. Baldereschi, Phys. Rev. B**50 (1994) 10715.**

11. R. Dovesi, R. Orlando, A. Erba, C. M. Zicovich-Wilson, B. Civalleri, S. Casassa, L. Maschio,
M. Ferrabone, M. De La Pierre, Ph. D’Arco, et al., Int. J. Quantum Chem.**114 (2014) 1287.**

12. L. Maschio, B. Kirtman, R. Orlando, and M. Rérat, J. Chem. Phys.**137 (2012) 204113.**

13. L. Maschio, B. Kirtman, M. Rérat, R. Orlando, and R. Dovesi, J. Chem. Phys.**139 (2013)**

167101.

14. K. Doll, Comput. Phys. Commun.**137 (2001) 74.**

16. K. Doll, R. Dovesi, and R. Orlando, Theor. Chem. Acc.**112 (2004) 394.**

17. K. Doll, R. Dovesi, and R. Orlando, Theor. Chem. Acc.**115 (2006) 354.**

18. S. de Gironcoli, S. Baroni, and R. Resta, Phys. Rev. Lett.**62 (1989) 2853.**

19. N. A. Hill and U. Waghmare, Phys. Rev. B**62 (2000) 8802.**

20. X. Wu, D. Vanderbilt, and D. Hamann, Phys. Rev. B**72 (2005) 035105.**

21. R. D. King-Smith and D. Vanderbilt, Phys. Rev. B**47 (1993) 1651.**

22. R. Resta, Rev. Mod. Phys.**66 (1994) 899.**

23. Y. Noël, M. Llunell, R. Orlando, Ph. D’Arco, and R. Dovesi, Phys. Rev. B**66 (2002) 214107.**

24. M. Catti, Y. Noël, and R. Dovesi, J. Phys. Chem. Solids**64 (2003) 2183.**

25. A. Erba, K. E. El-Kelany, M. Ferrero, I. Baraille, and M. Rérat, Phys. Rev. B**88 (2013) 035102.**

26. A. Erba, M. Ferrabone, J. Baima, R. Orlando, M. Rérat, and R. Dovesi, J. Chem. Phys.**138**

(2013) 054906.

27. B. Civalleri, P. D’Arco, R. Orlando, and R. D. V. R. Saunders, Chem. Phys. Lett.**348 (2001)**

131.

28. A. Mahmoud, A. Erba, K. E. El-Kelany, M. Rérat, and R. Orlando, Phys. Rev. B**89 (2014)**

045103.

29. K. E. El-Kelany, A. Erba, P. Carbonnière, and M. Rérat, J. Phys.-Condens. Mat.**26 (2014)**

205401.

30. K. E. El-Kelany, P. Carbonnière, A. Erba, and M. Rérat, J. Phys. Chem. C**119 (2015) 8966.**

31. J. Baima, A. Erba, R. Orlando, M. Rérat, and R. Dovesi, J. Phys. Chem. C**117 (2013) 12864.**

32. V. Lacivita, A. Erba, Y. Noël, R. Orlando, Ph. D’Arco, and R. Dovesi, J. Chem. Phys.**138**

(2013) 214706.

33. K. Doll, Mol. Phys.**108 (2010) 223.**

34. P. Otto, Phys. Rev. B**45 (1992) 10876.**

35. B. Champagne, J. G. Fripiat, and J. André, J. Chem. Phys.**96 (1992) 8330.**

36. P. Otto, F. L. Gu, and J. Ladik, J. Chem. Phys.**110 (1999) 2717.**

37. B. Kirtman, F. L. Gu, , and D. M. Bishop, J. Chem. Phys.**113 (2000) 1294.**

38. D. M. Bishop, F. L. Gu, and B. Kirtman, J. Chem. Phys.**114 (2001) 7633.**

39. M. Ferrero, M. Rérat, R. Orlando, and R. Dovesi, J. Comput. Chem.**29 (2008) 1450.**

40. M. Ferrero, M. Rérat, B. Kirtman, and R. Dovesi, J. Chem. Phys.**129 (2008) 244110.**

41. M. Ferrero, M. Rérat, R. Orlando, and R. Dovesi, J. Chem. Phys.**128 (2008) 014110.**

42. K. Kudin, R. Car, and R. Resta, J. Chem. Phys.**126 (2007) 234101.**

43. A. Izmaylov and G. Scuseria, Phys. Rev. B**77 (2008) 165131.**

44. V. R. Saunders, C. Freyria Fava, R. Dovesi, L. Salasco, and C. Roetti, Mol. Phys.**77 (1992)**

629.

*45. P. Pulay, Analytical Derivative Methods in Quantum Chemistry, John Wiley & Sons, Inc.,*

TSa(2007), pp. 241–286.

*46. J. F. Nye, Physical Properties of Crystals, Oxford University Press, Oxford (1957).*
47. J. P. Perdew, K. Burke, and M. Ernzerhof, Phys. Rev. Lett.**77 (1996) 3865.**

48. R. Dovesi, V. R. Saunders, C. Roetti, R. Orlando, C. M. Zicovich-Wilson, F. Pascale, K. Doll, N. M. Harrison, B. Civalleri, I. J. Bush, et al., CRYSTAL14 User’s Manual, Università di Torino, Torino (2014),http://www.crystal.unito.it.

49. R. Orlando, M. Ferrero, M. Rérat, B. Kirtman, and R. Dovesi, J. Chem. Phys.**131 (2009)**

184105.

50. V. Lacivita, M. Rérat, R. Orlando, M. Ferrero, and R. Dovesi, J. Chem. Phys.**136 (2012)**